WEAR OF ααα-ALUMINA IN HOT STEAM UP TO 300ºCm2d/Proceedings_M2D2017/... · Proceedings of the...
Embed Size (px)
Transcript of WEAR OF ααα-ALUMINA IN HOT STEAM UP TO 300ºCm2d/Proceedings_M2D2017/... · Proceedings of the...
Proceedings of the 7th International Conference on Mechanics and Materials in Design
Albufeira/Portugal 11-15 June 2017. Editors J.F. Silva Gomes and S.A. Meguid.
Publ. INEGI/FEUP (2017)
PAPER REF: 6421
WEAR OF αααα-ALUMINA IN HOT STEAM UP TO 300ºC
, Roman Ehrke, Mathias Woydt
Federal Institute for Materials Research and Testing (BAM), Berlin, Germany (*)Email: [email protected]
Selfmated α-alumina sliding couples have been investigated under oscillating sliding at 100 N
load in different humidity conditions in air as well as in hot steam up to temperatures of
300°C and ambient pressures up to 4 bar. The results show that the wear behaviour is directly
dependent on the amount of water in the environment. Two competing wear mechanisms are
identified: 1) abrasion is predominant in the low water vapour regime i.e. dry air whereas 2)
tribochemical wear is predominant, if enough water is available to form aluminium
hydroxide, i.e. in moist air and steam.
Keywords: α-alumina, wear, steam, temperature, abrasion.
According to the calculations of French company EXOES, the use of waste heat from exhaust
gases in cars and especially in trucks corresponds to possible energy savings in the range of 5
- 15 %, due to less fuel consumption. This relates to a corresponding reduction of the
emission of the green house gas CO2. Technological solutions in this field are manifold, one
of them is steam expansion using waste heat from the exhaust gas and converting it into
electrical energy by a piston expander. The development of improved materials and lubricants
for further increasing the efficiency needs testing devices suitable for steam environment.
This paper describes wear testing of alumina in water vapour atmosphere hence in laboratory
air as well as in steam up to temperatures of 300°C and 4 bar ambient pressure.
RESULTS AND CONCLUSIONS
When sliding against itself, wear of α-alumina is determined by the chemical equilibrium as
stated by the following equation:
Al2O3 + H2O � 2 AlOOH ∆G = -2.46·104 J
This equation has a negative Gibbs energy of formation at normal conditions of 25°C and 1
bar. Hence, in presence of water, Aluminium hydroxide in the form of Diaspore is formed and
is the stable phase. The Gibb’s energy of formation stays negative up to a temperature of
about 205°C and 1 bar ambient pressure. According to the equation above the thermodynamic
stability of the hydroxide phase is of crucial importance for the wear behaviour of selfmated
alumina. Corundum is a phase of relatively high hardness of 2035 Vickers, whereas Diaspore
has a much lower hardness of only about 1000 Vickers. Due to this difference the wear
behaviour of alumina will depend on the amount of water present in the environment which
can be seen in Fig. 1. The rough surface on the left side (Fig1a) is characteristic for
predominantly abrasive wear. This is typical for wear of α-alumina under the conditions of
low water content in the environment and relatively high coefficients of wear (Kong, 1992).
Topic-F: Tribology and Surface Engineering
Fig. 1 - SEM micrographs of wear scars after 100,000 cycles under dry sliding at
200°C, a) in air, b) in steam
In high water vapour or steam environments, especially above 100°C, the chemical formation
of hydroxide in the sliding interface causes a much smoother, less abraded surface with
distinct lower wear coefficients characterized by predominantly tribochemical wear, see Fig
Fig. 2 - Wear coefficient as function of temperature
The amount of water in the environment determines how much hydroxide is formed.
Consequently, the wear is predominantly abrasive with high wear rates if water content in the
environment is low (dry air). With increasing water content (moist air or hot steam) wear
becomes tribo-chemically modified due to the formation of hydroxide phase AlOOH causing
lower wear rates. This is seen in Fig 2, where wear rates increase with temperature
corresponding to decreasing relative humidity. In water rich atmosphere it stays low due to
the stability of hydroxide up to elevated temperatures. This is also observed during sliding in
-Kong H, Ashby M F. Wear mechanisms in brittle solids, Acta metall. mater.,1992, 40
(11), pp. 2907-2920.